Fabrication and Characterization of Anodic Titanium Oxide Nanotube Arrays of Controlled Length for Highly Efﬁcient Dye-Sensitized Solar Cells Chien-Chon Chen, † Hsien-Wen Chung, † Chin-Hsing Chen, † Hsueh-Pei Lu, † Chi-Ming Lan, † Si-Fan Chen, † Liyang Luo, †,‡ Chen-Shiung Hung, ‡ and Eric Wei-Guang Diau* ,† Department of Applied Chemistry and Institute of Molecular Science, National Chiao Tung UniVersity, No. 1001, Ta Hsueh Road, Hsinchu 300, Taiwan, and and Institute of Chemistry, Academia Sinica, Taipei 115, Taiwan ReceiVed: July 16, 2008; ReVised Manuscript ReceiVed: September 2, 2008 The performance of dye-sensitized solar cells (DSSC), made of highly ordered anodic titanium oxide (ATO) nanotube (NT) arrays produced directly on Ti foil, depends on the length of these arrays. We controlled these lengths L from 4 to 41 µm while varying the concentration (0.1, 0.25, 0.5, and 0.8 wt %) of the electrolyte (NH 4 F) in ethylene glycol in the presence of H 2 O (2 vol %) with anodization for various periods (t ) 0.5-8 h). The compact and bundle layers introduced during anodization were effectively removed upon simple ultrasonic cleaning in deionized water containing submicrometer particles of Al 2 O 3 in a small proportion. The photovoltaic performance of the NT-DSSC devices (NH 4 F at 0.5 wt %) made of ATO ﬁlms, as prepared, increased from 3.0% to 5.2% as L was increased from 6 µm(t ) 0.5 h) to 30 µm(t ) 8 h). After treatment of the ATO ﬁlms with TiCl 4 in a two-step annealing process, the optimized NT-DSSC device attained an overall efﬁciency of 7.0% power conversion. 1. Introduction Following the pioneering work of Gra ¨tzel and co-workers, 1 dye-sensitized solar cells (DSSC) have received much attention as an economical energy conversion device. A typical DSSC device contains a light-harvesting layer on a working electrode (anode) and a Pt-coated layer on a counter electrode (cathode); both electrodes are made of a transparent conducting oxide (TCO) substrate; an iodine-based electrolyte ﬁlls the space between the anode and the cathode to serve as a redox mediator in a sandwich-type structure. As a light-harvesting layer, a photosensitizer, typically a ruthenium complex such as N3 or N719 dye, is chemisorbed onto the surface of a nanocrystalline thin ﬁlm of TiO 2 . When this photosensitizer absorbs sunlight, electrons are injected into the conduction band of the semicon- ductor layer, which results in a separation of electrons (in the TiO 2 layer) and holes (dye cations); the electrons proceed to the anode while the holes are transported by the redox species to the cathode to complete the photoelectrochemical cycle and to do external work. The electron-collecting layer (anode) of a DSSC is traditionally composed of randomly packed TiO 2 nanoparticles (NP). With sunlight irradiating the transparent anode (front illumination), the greatest efﬁciency (η) of conver- sion into photovoltaic power of a NP-DSSC device has reached ∼11%. 2–6 A great advantage of a NP-DSSC is that nanoporous TiO 2 ﬁlms have a large surface area for dye adsorption, but diffusion, limited by traps, for electron transport in NP-DSSC impedes the efﬁciency of conversion of light to electricity. 7,8 To improve the efﬁciency of charge collection by promoting both more rapid electron transport and slower charge recombination, several methods with TiO 2 ﬁlms constructed of oriented one-dimen- sional (1D) nanostructures have been established. For instance, DSSC based on one-dimensional TiO 2 nanowires have been reported; 9,10 1D TiO 2 nanotubes (NT) have been synthesized using the sol-gel method 11–13 and potentiostatic anodization. 8,14–20 Gra ¨tzel and co-workers reported a back-illuminated NP-DSSC with a cell performance η ) 7.2%. 21 Because substantial light scattering at the Pt-coated counter electrode and light absorption by the iodine-based electrolyte adversely affect the performance, the back-illuminated NP-DSSC has an efﬁciency signiﬁcantly smaller than that of its front-illuminated counterpart (η ) 9.9%); maximum values occur at a TiO 2 ﬁlm thickness of 14 µm in both cases. 21 For NT-DSSC, perpendicularly aligned and highly ordered anodic titanium oxide (ATO) NT arrays are prepared either on a TCO glass, using combined sputtering/anodization 8 or a ﬁlm detachment, 20 or on a nontransparent Ti metal surface, using direct anodization. 14–19 Front illumination is feasible for only the former case, but poor adhesion between the ATO barrier layer and the TCO layer limits the length of ATO NT arrays. Although illumination from the back suffers from the speciﬁed disadvantages, NT-DSSC with ATO NT arrays on Ti foil as working electrodes have many important intrinsic features that outperform conventional NP-DSSC. First, the efﬁciency of charge collection of NT ﬁlms has been proved to be much better than that of NP ﬁlms because of the 1D nature of the former with a much smaller rate of charge recombination; 16 this intrinsic advantage of NT-DSSC signiﬁcantly promotes its cell performance with increasing tube length up to 20 µm as reported by Grimes and co-workers. 17 Second, the efﬁciency of light harvesting by NT ﬁlms is much better than that of NP ﬁlms because the former have a stronger light scattering effect; 16 for a traditional, highly efﬁcient NP-DSSC, adding an additional TiO 2 layer of larger particles (size ∼400 nm) 2,3,21 or increasing the haze factor 5,6 was required to increase the light scattering, whereas this effect is a natural property of a NT-DSSC. Third, the anode fabrication of a NT-DSSC is much simpler and cheaper than that of a NP-DSSC. Direct anodization of a Ti * Corresponding author. Fax: (886)-03-572-3764. E-mail: diau@ mail.nctu.edu.tw. † National Chiao Tung University. ‡ Academia Sinica. J. Phys. Chem. C 2008, 112, 19151–19157 19151 10.1021/jp806281r CCC: $40.75 2008 American Chemical Society Published on Web 11/08/2008
Fabrication and Characterization of Anodic Titanium Oxide Nanotube Arrays of ControlledLength for Highly Efficient Dye-Sensitized Solar Cells
Si-Fan Chen,† Liyang Luo,†,‡ Chen-Shiung Hung,‡ and Eric Wei-Guang Diau*,†
Department of Applied Chemistry and Institute of Molecular Science, National Chiao Tung UniVersity,No. 1001, Ta Hsueh Road, Hsinchu 300, Taiwan, and and Institute of Chemistry, Academia Sinica,Taipei 115, Taiwan
ReceiVed: July 16, 2008; ReVised Manuscript ReceiVed: September 2, 2008
The performance of dye-sensitized solar cells (DSSC), made of highly ordered anodic titanium oxide (ATO)nanotube (NT) arrays produced directly on Ti foil, depends on the length of these arrays. We controlled theselengths L from 4 to 41 µm while varying the concentration (0.1, 0.25, 0.5, and 0.8 wt %) of the electrolyte(NH4F) in ethylene glycol in the presence of H2O (2 vol %) with anodization for various periods (t ) 0.5-8h). The compact and bundle layers introduced during anodization were effectively removed upon simpleultrasonic cleaning in deionized water containing submicrometer particles of Al2O3 in a small proportion.The photovoltaic performance of the NT-DSSC devices (NH4F at 0.5 wt %) made of ATO films, as prepared,increased from 3.0% to 5.2% as L was increased from 6 µm (t ) 0.5 h) to 30 µm (t ) 8 h). After treatmentof the ATO films with TiCl4 in a two-step annealing process, the optimized NT-DSSC device attained anoverall efficiency of 7.0% power conversion.
Following the pioneering work of Gratzel and co-workers,1
dye-sensitized solar cells (DSSC) have received much attentionas an economical energy conversion device. A typical DSSCdevice contains a light-harvesting layer on a working electrode(anode) and a Pt-coated layer on a counter electrode (cathode);both electrodes are made of a transparent conducting oxide(TCO) substrate; an iodine-based electrolyte fills the spacebetween the anode and the cathode to serve as a redox mediatorin a sandwich-type structure. As a light-harvesting layer, aphotosensitizer, typically a ruthenium complex such as N3 orN719 dye, is chemisorbed onto the surface of a nanocrystallinethin film of TiO2. When this photosensitizer absorbs sunlight,electrons are injected into the conduction band of the semicon-ductor layer, which results in a separation of electrons (in theTiO2 layer) and holes (dye cations); the electrons proceed tothe anode while the holes are transported by the redox speciesto the cathode to complete the photoelectrochemical cycle andto do external work. The electron-collecting layer (anode) of aDSSC is traditionally composed of randomly packed TiO2
nanoparticles (NP). With sunlight irradiating the transparentanode (front illumination), the greatest efficiency (η) of conver-sion into photovoltaic power of a NP-DSSC device has reached∼11%.2–6
A great advantage of a NP-DSSC is that nanoporous TiO2
films have a large surface area for dye adsorption, but diffusion,limited by traps, for electron transport in NP-DSSC impedesthe efficiency of conversion of light to electricity.7,8 To improvethe efficiency of charge collection by promoting both more rapidelectron transport and slower charge recombination, severalmethods with TiO2 films constructed of oriented one-dimen-
sional (1D) nanostructures have been established. For instance,DSSC based on one-dimensional TiO2 nanowires have beenreported;9,10 1D TiO2 nanotubes (NT) have been synthesizedusing the sol-gel method11–13 and potentiostatic anodization.8,14–20
Gratzel and co-workers reported a back-illuminated NP-DSSCwith a cell performance η ) 7.2%.21 Because substantial lightscattering at the Pt-coated counter electrode and light absorptionby the iodine-based electrolyte adversely affect the performance,the back-illuminated NP-DSSC has an efficiency significantlysmaller than that of its front-illuminated counterpart (η ) 9.9%);maximum values occur at a TiO2 film thickness of 14 µm inboth cases.21 For NT-DSSC, perpendicularly aligned and highlyordered anodic titanium oxide (ATO) NT arrays are preparedeither on a TCO glass, using combined sputtering/anodization8
or a film detachment,20 or on a nontransparent Ti metal surface,using direct anodization.14–19 Front illumination is feasible foronly the former case, but poor adhesion between the ATO barrierlayer and the TCO layer limits the length of ATO NT arrays.
Although illumination from the back suffers from thespecified disadvantages, NT-DSSC with ATO NT arrays on Tifoil as working electrodes have many important intrinsic featuresthat outperform conventional NP-DSSC. First, the efficiencyof charge collection of NT films has been proved to be muchbetter than that of NP films because of the 1D nature of theformer with a much smaller rate of charge recombination;16 thisintrinsic advantage of NT-DSSC significantly promotes its cellperformance with increasing tube length up to 20 µm as reportedby Grimes and co-workers.17 Second, the efficiency of lightharvesting by NT films is much better than that of NP filmsbecause the former have a stronger light scattering effect;16 fora traditional, highly efficient NP-DSSC, adding an additionalTiO2 layer of larger particles (size ∼400 nm)2,3,21 or increasingthe haze factor5,6 was required to increase the light scattering,whereas this effect is a natural property of a NT-DSSC. Third,the anode fabrication of a NT-DSSC is much simpler andcheaper than that of a NP-DSSC. Direct anodization of a Ti
† National Chiao Tung University.‡ Academia Sinica.
J. Phys. Chem. C 2008, 112, 19151–19157 19151
10.1021/jp806281r CCC: $40.75 2008 American Chemical SocietyPublished on Web 11/08/2008
foil in one step produces a blank TiO2 film ready to act as aworking electrode for a NT-DSSC, whereas making a blankTiO2 film for a NP-DSSC requires multiple coatingssat leasttwo layers of TiO2 NP coating on an expensive TCO substrate.Furthermore, calcination of the NT/Ti anode at a high temper-ature makes it ready to be fabricated into a flexible NT-DSSCdevice with a transparent conductive plastic cathode (ITO/PEN).Gratzel and co-workers reported an efficiency of 3.6% photo-voltaic conversion for a flexible NT-DSSC made of ATO NTfilms of thickness 14 µm with a solvent-free ionic liquidelectrolyte.19
Even though the TiO2 NT arrays possess the advantages ofgreater efficiency of charge collection and stronger lightscattering than their NP-based counterparts,16 producing longertubes on a larger area involves formation of a bundle layer inthe films, leading to cracking of films that are easily peeledfrom the Ti substrate. To resolve this problem, Frank and co-workers22 removed solvent liquids from the mesopores of thearrays with supercritical CO2, so producing NT films free ofbundles and cracks for NT-DSSC applications, but the smalllength of the TiO2 NT arrays (L ) 6.1 µm) limited the efficiencyof power conversion of the device (η ) 1.9%).22 The greatestreported efficiency of NT-DSSC under backside illuminationis 6.89%.17
In the present work, we controlled the lengths of ATO NTfrom 4 to 41 µm while varying the concentration of NH4Felectrolyte in ethylene glycol (EG) with anodization for variousperiods. The unwanted surface deposits of the films introducedduring anodization were effectively removed simply uponultrasonic cleaning in deionized water containing Al2O3 assubmicrometer particles in a small proportion. We observed asystematic variation of the photovoltaic performance of the NT-DSSC devices as a function of tube length. After the ATO films
were treated with TiCl4 and annealed in two steps, we foundthat, with an appropriate redox electrolyte and an improvedcounter electrode, the optimized NT-DSSC device reaches anoverall efficiency of 7.0% power conversion.
2. Experimental Section
We fabricated ordered nanochannel arrays of ATO films at25 °C on anodizing titanium (Ti) foil (Aldrich, 99.7% purity)as circular discs (diameter ∼50 mm) at a constant voltage of60 V.17,23 The electrolyte solutions contained ammonium fluoride(NH4F, 99.9%; 0.15, 0.25, 0.5, and 0.8 wt %) in EG in thepresence of H2O (2 vol %, pH ) 6.8) with anodization for variedperiods (t ) 0.5-8 h). To crystallize amorphous TiO2 into itsanatase phase, we annealed the samples to 450 °C. Parts a andb of Figure 1 show SEM images of the ATO films subjected toannealing in one and two steps, respectively. For the two-stepprocess, the ATO films were first rinsed with ethanol, dried inair, and annealed at 150 °C for 2 h to remove organic solvents,and were then crystallized at 450 °C for another 3 h in an airfurnace. After one-step annealing directly at 450 °C, the ATOfilm suffered severe cracking that resulted in the film becomingeasily peeled from the Ti-foil substrate, as demonstrated in theinset of Figure 1a. The inset of Figure 1b shows the satisfactoryquality of the ATO films of large area from the two-stepannealing.
When the ATO NT were produced with the electrolyte atlarge concentrations or with protracted anodization, we observedthe formation of compact layers on the surface of the ATO films(Figure 2a); a bundle layer was observed (Figure 2b) at a smalleranodization period, as Frank and co-workers reported.22 Becauseof the robust structure of the NT arrays and the loose structureof the surface debris, the unwanted deposits on the ATO surface
Figure 1. SEM images of ATO films undergoing (a) a one-step annealing and (b) a two-step annealing. The insets show specimen pictures of thecorresponding ATO films: the one-step process leads to creaking of the films that easily peeled from the Ti substrate, whereas the two-step processyields films of satisfactory quality and ready to use.
Figure 2. SEM images of ATO NT covered with (a) a compact layer and (b) a bundle layer before ultrasonic cleaning.
19152 J. Phys. Chem. C, Vol. 112, No. 48, 2008 Chen et al.
introduced during anodization can be effectively removed withultrasonic vibration of the ATO films in deionized watercontaining a small proportion of Al2O3 particles of average size300 nm. Parts a and b of Figure 3 show top and side views ofSEM images of ATO films after ultrasonic cleaning thatcompletely removed the disordered clumps, but the length ofthe tube decreased from 36 to 30 µm. Afterward, the sampleswere again washed with ethanol, dried in air, and heated to 100°C for 10 min followed by annealing at 450 °C for 30 min.
The surface roughness of ATO films was measured with asurface profiler (R-step; KOSAKA, ET-4000); these films werecharacterized with parameters for average roughness (Ra), root-mean-square roughness (Rq), and average maximum height ofthe profile (Rz). For a typical ATO film, these roughnessparameters before ultrasonic treatment were Ra ) 0.46 µm, Rq) 0.53 µm, and Rz ) 2.91 µm; the parameters after thattreatment were Ra ) 0.80 µm, Rq ) 0.93 µm, and Rz ) 4.38µm. We therefore estimate the uncertainty of the ATO filmthickness to be (2 µm according to the measured 2Rq values(two standard errors). The morphology of the ATO films wasdetermined with a scanning electron microscope (SEM; JEOL6500) and the composition with X-ray diffraction (XRD; PhilipsX’Pert Pro).
To characterize the photovoltaic performance of the NT-DSSC devices, we immersed the ATO films (typical size 1.2× 2.0 cm2) in an ethanol solution containing N3 (0.5 mM,Solaronix, Switzerland) at 50 °C for 8 h to absorb sufficientN3 dye for light harvesting; the N3/ATO films served as aworking electrode (anode). A fluorine-doped tin oxide (FTO;
30 Ω/sq, Sinonar, Taiwan) glass (typical size 1.0 × 2.0 cm2)coated with Pt particles by sputtering served as a counterelectrode (cathode). To fabricate the NT-DSSC device, weassembled the two electrodes into a cell of sandwich type andsealed it with a hot-melt film (SX1170, Solaronix, thickness 25µm); a thin layer of electrolyte was introduced into the spacebetween the two electrodes.17,18 A typical redox electrolytecontained lithium iodide (LiI, 0.1 M), diiodine (I2, 0.01 M),4-tert-butylpyridine (TBP, 0.5 M), butyl methyl imidazoliumiodide (BMII, 0.6 M), and guanidinium thiocyanate (GuNCS,0.1 M) in a mixture of acetonitrile (CH3CN, 99.9%) andvaleronitrile (n-C4H9CN, 99.9%) (v/v ) 15/1).
The amount of N3 dye absorbed on the ATO films wasmeasured with a UV-visible-NIR spectrophotometer (JASCOV-570) equipped with an integrating sphere (JASCO ISN-470).Measurements of IV curves were made with a digital sourcemeter (Keithley 2400, computer-controlled) with the device
Figure 3. SEM images of ATO NT after ultrasonic cleaning: (a) top view and (b) side view. The inset of (a) shows the enlarged pattern of theATO NT arrays.
Figure 4. Length of ATO NT (L) as a function of anodization period(t) at various NH4F concentrations (wt %) as indicated; the correspond-ing side-view SEM images showing the L values of each datum aregiven in the Supporting Information.
Figure 5. (a) Absorption spectra of ATO films sensitized with N3dye at various tube lengths produced with NH4F (0.5 wt %). (b)Current-voltage characteristics of NT-DSSC devices fabricated usingthe corresponding ATO films (a) under simulated AM-1.5 solarillumination (100 mW cm-2) and active area 0.28 cm2.
Anodic TiO2 Nanotube Arrays for DSSC J. Phys. Chem. C, Vol. 112, No. 48, 2008 19153
under one-solar AM-1.5 irradiation from a solar simulator(Newport-Oriel 91160) calibrated with a Si-based reference cell(Hamamatsu S1133) containing an IR-cut filter (KG5) to correctthe spectral mismatch of the lamp.24 The NT-DSSC devices were
operated with illumination on the back side and the transparentcounter electrode masked with a black plastic tape of the samesize with a round hole to allow the actively illuminated area,0.28 cm2, for all measurements.25
The incident monochromatic photon-to-current conversionefficiency (IPCE) measurements were carried out with a home-built system, which includes a Xe lamp (PTi A-1010, 150 W),a monochromator (Dongwoo DM150i, 1200 gr/mm blazed at500 nm), and a source meter (Keithley 2400, computer-controlled). A standard Si photodiode (ThorLabs FDS1010) wasused as a reference to calibrate the power density of the lightsource at each wavelength so that the IPCE(λ) of the NT-DSSCdevice can be obtained according to the following equation
IPCE(λ)) IPCEref(λ) ·JDSSC(λ)
where the IPCEref(λ) of the Si photodiode is known from acalibration, and the current densities of the reference cell andthe NT-DSSC device, Jref(λ) and JDSSC(λ), were measured underthe same experimental conditions (excitation beam size ∼0.08cm2).
3. Results and Discussion
3.1. Growing ATO Films with Various Lengths of NTArrays. According to Grimes and co-workers,14,17 the formationof ATO NT involves fluoride ions: the lengths of these tubeswere proportional to the fluoride concentration and to theduration of anodization. We confirmed this correlation, but thetubes adhered more weakly to the substrate when the tubes grewlonger. To discover optimal conditions for long tubes tightlygrown on the substrate, we used NH4F electrolyte in EG at fourconcentrations to anodize Ti foil with anodization for variousdurations. Figure 4 shows the variation of length of TiO2 NTas a function of period of anodization (the corresponding SEMimages of each datum showing the lengths of the tubes are givenin the Supporting Information, Figures S1-S4); the lengthincreased with increasing duration of anodization and F-
Figure 6. Variation of photovoltaic parameters JSC, VOC, FF, and η,as a function of tube length (L); these data were obtained from analysisof IV curves in Figure 5b and summarized in Table 1.
TABLE 1: Photovoltaic Performance of NT DSSC as aFunction of Tube Length (L) under AM-1.5 Illumination(Power 100 mW cm-2) and Active Area 0.28 cm2a
a Values obtained for ATO films without TiCl4 treatment; thecounter electrodes were not optimized.
Figure 7. SEM images of ATO NT after treatments with TiCl4: (a) and (c) top and side views with annealing temperature 350 °C; (b) and (d) topand side views with annealing temperature 450 °C. The scale bars represent a length of 100 nm.
19154 J. Phys. Chem. C, Vol. 112, No. 48, 2008 Chen et al.
concentration. Our results indicate that the maximum lengthsof NT with effective adhesion to the Ti substrate are 16, 20,30, and 41 µm for NH4F concentrations 0.15, 0.25, 0.5, and0.8 wt % in EG, respectively. At small [F-], the cracking wasnot severe, but the rate of tube growth was so small as to leadto formation of heavier clumps on the surface of the films. Atlarge [F-], even though the rate of tube growth was muchincreased, cracking also became significant, which causes pooreradhesion of the tubes to the substrate. As a compromise, weused ATO films grown with [NH4F] at 0.5 wt % for variousperiods of anodization to investigate the dependence of thephotovoltaic performance of NT-DSSC devices on length.
3.2. Photovoltaic Performance of the Devices with NTArrays of Varied Lengths. The ability of the N3 dyechemisorbed on ATO films was examined with absorptionspectra as shown in Figure 5a, in which the absorbance of thedye increases upon L increasing from 6 to 18 µm but variesinsignificantly for L above 18 µm because of the saturation ofthe instrument (Supporting Information, Figure S5). The absorp-tion maximum of the dye shifts slightly from 530 nm for shorter
tubes to 536 nm for longer tubes, together with a broad shoulderextending to greater wavelengths for the longer tubes. Thisspectral feature of the increased dye loading in longer tubesmight be due to a saturation effect and/or due to the increase ofmolecular interaction that results in the broader shoulder towardthe red part of the visible spectra. These N3/ATO films werefabricated into NT-DSSC devices of which the correspondingIV curves are shown in Figure 5b. We show the measuredphotovoltaic parameters of these devices in Figure 6; thecorresponding values are summarized in Table 1, whichdemonstrates that the current density at short circuit (JSC in mAcm-2), the voltage at open circuit (VOC in V), the fill factor (FF),and the efficiency of power conversion (η ) JSC ·VOC ·FF/Pin
with Pin ) 100 mW cm-2) vary with the tube length (L). Theresults display a notably systematic trend for JSC, such that thecurrent density increases significantly from JSC ) 6.4 mA cm-2
at L ) 6 µm to JSC ) 12.5 mA cm-2 at L ) 30 µm becauselonger tubes offer a larger surface area on which the dyemolecules adsorb.
Our results also show a systematic trend with both VOC andFF decreasing upon increasing tube length. Because the extentof the increase in JSC was much greater than the extent of thedecrease in VOC and FF, the overall efficiency of conversion ofphotons to current exhibited a systematic increase from η )3.0% at L ) 6 µm to η ) 5.2% at L ) 30 µm. A negativedependence of cell performance on length in both VOC and FFis unambiguously shown in Figure 6, indicating that chargerecombination might be important at the interface between theelectrode and the electrolyte.26,27 The source of charge recom-bination might have been the cracking of the films (Figure 1b),which became more significant for films of tubes of increasinglength. To remedy this problem, we further treated the ATOfilms with TiCl4.28,29
3.3. Photovoltaic Performance on TiCl4 Treatments ofATO Films. The effect of the TiCl4 treatment on ATO films isreported to increase the amount of dye loading and hence toenhance the photocurrent of the device.18 In particular, it hasbeen shown that the TiCl4 treatment in a front-illuminated NT-DSSC increases the roughness of the tube walls and thusimproves the cell performance through an increased effectivesurface area for dye adsorption.8,18,20 The dye-loading experi-ments have confirmed that the amount of adsorbed N3 dye on
Figure 8. Current-voltage characteristics of NT-DSSC devicesfabricated using the ATO films treated with TiCl4 as shown in Figure7 under simulated AM-1.5 solar illumination (100 mW cm-2) and activearea 0.28 cm2. The dashed curve shows the results of an ATO film nottreated with TiCl4 for comparison.
Figure 9. (a) Photocurrent and (b) IPCE spectra of the TiCl4-treatedNT-DSSC (circles) and the Si reference cell (dashed curves) measuredat the same experimental conditions.
Figure 10. Current-voltage characteristics of NT-DSSC devicesfabricated using four electrolytes: (a) electrolyte A, (b) electrolyte B,(c) electrolyte C, and (d) electrolyte D under simulated AM-1.5 solarillumination (100 mW cm-2) and active area 0.28 cm2. Three to fourindependent measurements were conducted with the same ATO films.The compositions of the electrolytes are summarized in Table 2.
Anodic TiO2 Nanotube Arrays for DSSC J. Phys. Chem. C, Vol. 112, No. 48, 2008 19155
a TiCl4-treated ATO film is larger than that adsorbed on anuntreated ATO film (Supporting Information, Figures S6 andS7). We further tested the effect of the TiCl4 treatments in aback-illuminated NT-DSSC by varying the immersion temper-atures and periods and the annealing temperatures. Accordingto those tests, the best condition was to treat TiCl4 twice at 50°C; for the first treatment, the films were immersed in TiCl4(aq)
(0.1 M, 1.5 h) followed by appropriate rinsing and drying (300°C, 30 min); for the second treatment, the films were immersedin TiCl4(aq) (0.1 M, 1.5 h) again and then annealed at either 350or 450 °C for 30 min. Parts a/c and b/d of Figure 7 show topand side views of SEM images of the TiCl4-treated ATO films(L ) 19 µm) at annealing temperatures 350 and 450 °C,respectively. The two-step treatments of the ATO films withTiCl4 clearly formed compact TiO2 nanoparticles on the innerand outer surfaces of the NT so as to increase the surface areafor dye adsorption. The TiO2 nanoparticles produced at anannealing temperature of 350 °C were smaller than those formedat 450 °C.
After the ATO films treated with TiCl4 were sensitized withN3 dye, the N3/ATO films were fabricated into NT-DSSCtogether with an improved counter electrode.30 The effect ofTiCl4 treatment on cell performance is shown in Figure 8; theIV characteristic of an ATO film not treated with TiCl4 appearsas a dashed curve (JSC ) 13.8 mA cm-2; VOC ) 0.741 V; FF )0.58; η ) 5.9%) for comparison. After posttreatment of the ATOfilms with TiCl4, JSC, VOC, and FF of the NT-DSSC devicesincreased significantly, so improving the cell performance fromη ) 5.9% to η ) 7.0%. Both TiCl4-treated ATO films havesimilar values of η. Although the values of VOC are similar, thevalue of JSC for the film annealed at 350 °C is greater than thatfor annealing at 450 °C owing to larger surface area of theformer for enhanced dye loading. A higher temperature ofannealing of the latter might aid nucleation of the nanoparticularTiO2 into the anatase phase for improved electron transport andhence an increased fill factor of the device. These two effectsappeared to balance each other, such that almost the same cellperformance was obtained for the two-step TiCl4 treatments attwo annealing temperatures.
The photocurrent action (IPCE) spectrum of the TiCl4-treatedNT-DSSC device was obtained from a calibrated experiment.Figure 9a shows the photocurrents of NT-DSSC (circles) andthe Si reference cell (dashed curve), which were obtained underthe same experimental conditions. Because the IPCEref(λ) ofthe reference cell was known (dashed curve in Figure 9b), theIPCE(λ) of the NT-DSSC device can be evaluated accordingto eq 1, and the results are shown as circles in Figure 9b. TheIPCE spectrum exhibits a maximum around 530 nm, which issimilar to the feature of the absorption spectra of the N3/ATOfilms shown in Figure 5a. Furthermore, our IPCE spectrum isalso similar to the IPCE spectrum of a back-illuminated NP-DSSC device with η ) 7.2%.21 It was pointed out21 that the
IPCE values of a back-illuminated DSSC device are lower thanthose of its front-illuminated counterpart owing to the absorptionof the I3
- electrolyte that cuts the incident light significantlybelow 500 nm.
To save time in loading the dye onto the ATO films, we usedthe N3 dye with immersion period 8 h, whereas Grimes andco-workers17 used N719 dye with immersion period 48 h, andthis leads to a lower VOC value being observed.31 The durationof growth of an ATO film with L ) 20 µm was much smallerin our case (3-4 vs 24 h), which might be an important concernfor future commercialization of a NT-DSSC.
3.4. Effect of the Redox Electrolytes. Because sunlight istransmitted through the redox electrolyte before being absorbedby dye molecules in a back-illuminated NT-DSSC device, thecomposition of the electrolyte might play a role in the cellperformance. For example, Grimes and co-workers reported η) 5.44% for their back-illuminated NT-DSSC result with theelectrolyte solution composed of LiI (0.5 M), I2 (0.05 M), TBP(0.5 M), N-methylbenzimidazole (MBI, 0.6 M), and GuNCS(0.1 M) in methoxypropionitrile (MPN); their device suffersfrom a small FF value (0.43), which was attributed to a thickbarrier layer of the ATO film.14 The large concentrations of LiIand I2 in the electrolyte might obstruct significantly the incidentlight in a backside illumination device. The same groupsubsequently reported η ) 6.89% for an electrolyte containingI2 (0.01 M), MBI (0.5 M), BMII (0.6 M), and GuNCS (0.1 M)in MPN.17 Our tests indicate that this electrolyte still suffersfrom a small FF value, probably due to the large viscosity ofMPN; altering the MPN solvent to a cosolvent of acetonitrileand valeronitrile with a volume ratio 15:1 (electrolyte A in Table2) much improves the cell performance (η ) 5.9%). TBP inthe electrolyte is known to play an important role in increasingboth VOC and FF values through remedying the dye-uncoveredsurface of the ATO films.28 Recent investigations32,33 show thataddition of TBP containing Li+ ions in the electrolyte reducesthe surface positive charge, which shifts the conduction bandpotential of TiO2 toward negative and leads to the increase ofVOC. Furthermore, TBP suppressed the recombination betweenthe injected electrons and triiodide anions that leads to theincrease of VOC and FF.33,34 By replacement of the MBIcomponent with TBP (0.5 M) and addition of LiI (0.1 M) toincrease the iodine anions, the device made of electrolyte Bproduces much better cell performance than the device madeof electrolyte A (Table 2).
The IV characteristics of the NT-DSSC made of fourelectrolytes (A-D), repeated three to four times, are shown inFigure 10; the corresponding averaged photovoltaic parametersare summarized in Table 2. Electrolyte C, adopted from Gratzeland co-workers,21 was designed for both front- and back-illuminated NP-DSSC devices. The large concentration of I2
and lack of Li+ in electrolyte C lead to the decrease in both JSC
and VOC that causes device C to have a deteriorated cell
TABLE 2: Photovoltaic Performance of NT-DSSC at Four Compositions of Electrolytes under AM-1.5 Illumination (Power 100mW cm-2) and Active Area 0.28 cm2a
a All photovoltaic parameters were obtained from averaging three to four sets of the IV curves shown in Figure 10; the uncertaintiesrepresent two standard errors. b Additional component in electrolytes A-D contains guanidinium thiocyanate (GuNCS, 0.1 M) in a mixture ofacetonitrile and valeronitrile (volume ratio 15/1 for A and B, and 85/15 for C and D). c Electrolyte A contains no 4-tert-butylpyridine (TBP)but contains N-methylbenzimidazole (MBI, 0.5 M).
19156 J. Phys. Chem. C, Vol. 112, No. 48, 2008 Chen et al.
performance relative to device B (η ) 6.4% vs η ) 6.9%).Because the presence of Li+ ions might increase the amount ofTBP adsorption on TiO2 surface,32 lack of Li+ ions in electrolyteC could result in lower VOC as we have observed (Table 2).Increasing the concentration of I2 increases the concentrationof triiodide anions so increasing the hole transport mobility,but this effect is balanced in a back-illuminated device by theattenuation of the incident light in the visible region (λ < 500nm). However, the cell performance improved significantly withthe additions of 0.05 M LiI and 1.0 M BMII in electrolyte D,which is a new redox electrolyte for NP-DSSC reported byGratzel and co-workers.35 The performance of device D iscomparable to that of device B, which gives the best cellperformance for a back-illuminated NT-DSSC device.
In summary, we fabricated dye-sensitized solar cells basedon working electrodes made of highly ordered anodic titaniumoxide nanotube arrays of varied tube length directly formed onTi foil. The lengths of these ATO NT were controlled from 4to 41 µm while varying the concentrations of NH4F electrolyte(0.1, 0.25, 0.5, and 0.8 wt %) in EG in the presence of H2O (2vol %) for various periods (t ) 0.5-8 h) of anodization. Theunwanted surface deposits introduced during anodization wereeffectively removed simply with ultrasonic cleaning. Aftersensitization of the ATO film with N3 dye, the N3/ATO filmserved as a working electrode to fabricate a NT-DSSC device.We observed a systematic variation of the photovoltaic perfor-mance of NT-DSSC devices (with NH4F at 0.5 wt %) increasingfrom 3.0% to 5.2% as L was increased from 6 µm (t ) 0.5 h)to 30 µm (t ) 8 h). After posttreatment of ATO films withTiCl4 by annealing in two steps, the cell performance of theNT-DSSC device increased further to η ) 7.0% at L ) 19 µm.The best electrolyte tested for a back-illuminated device containsLiI (0.1 M), I2 (0.01 M), BMII (0.6 M), TBP (0.5 M), andGuNCS (0.1 M) in a mixture of acetonitrile and valeronitrile(v/v ) 15/1). We emphasize the significance of the present workfor the growth of ATO films with longer nanotubes at muchsmaller periods of anodization, which might be an importantconcern for future commercialization of NT-DSSC.
Acknowledgment. The National Science Council of theRepublic of China provided financial support through projectcontracts 96-2628-M-009-018-MY2 and 96-2627-M-009-005.Support from the MOE-ATU program and Niching IndustrialCorporation are also acknowledged.
Supporting Information Available: Side-view SEM imagesof the ATO films shown in Figure 4, absorption spectra of theN3/ATO films shown in Figure 5a, absorption spectra of dye-loading experiments, TEM images of Pt-sputtered patterns, andtransmission spectra of Pt-sputtered FTO substrates. Thisinformation is available free of charge via the Internet at http://pubs.acs.org.
References and Notes
(1) O’Regan, B.; Gratzel, M. Nature 1991, 353, 737.(2) Nazeeruddin, M. K.; Angelis, F. D.; Fantacci, S.; Selloni, A.;
Viscardi, G.; Liska, P.; Ito, S.; Takeru, B.; Gratzel, M. J. Am. Chem. Soc.2005, 127, 16835.
(3) Wang, Q.; Ito, S.; Gratzel, M.; Fabregat-Santiago, F.; Mora-Sero,I.; Bisquert, J.; Bessho, T.; Imai, H. J. Phys. Chem. B 2006, 110, 25210.
(4) Wei, M.; Konishi, Y.; Zhou, H.; Yanagida, M.; Sugihara, H.;Arakawa, H. J. Mater. Chem. 2006, 16, 1287.
(5) Koide, N.; Islam, A.; Chiba, Y.; Han, L. J. Photochem. Photobiol.,A 2006, 182, 296.
(25) Ito, S.; Nazeeruddin, M. K.; Liska, P.; Comte, P.; Charvet, R.;Pechy, P.; Jirousek, M.; Kay, A.; Zakeeruddin, S. M.; Gratzel, M. Prog.PhotoVolt.: Res. Appl. 2006, 14, 589.
(26) Ito, S.; Liska, P.; Comte, P.; Charvet, R.; Pechy, P.; Bach, U.;Schmidt-Mende, L.; Zakeeruddin, S. M.; Kay, A.; Nazeeruddin, M. K.;Gratzel, M. Chem. Commun. 2005, 4351.
(27) Bandaranayake, K. M. P.; Senevirathna, M. K. I.; Weligamuwa,P. M. G. M. P.; Tennakone, K. Coord. Chem. ReV. 2004, 248, 1277.
(28) Nazeeruddin, M. K.; Kay, A.; Rodicio, I.; Humphry-Baker, R.;Muller, E.; Liska, P.; Vlachopoulos, N.; Gratzel, M. J. Am. Chem. Soc.1993, 115, 6382.
(29) Barbe, C. J.; Arendse, F.; Comte, P.; Jirousek, M.; Lenzmann, F.;Shklover, V.; Gratzel, M. J. Am. Ceram. Soc. 1997, 80, 3157.
(30) Because the performance of a back-illuminated NT-DSSC is verysensitive to the quality of the counter electrode, we tested the cellperformance with the electrode made of highly transparent FTO glasssputtered by a thin layer of platinum. We found that the active area (0.28cm2) of the counter electrode of Pt sputtered for 14 s (power 10 W; targetsize 81 cm2; distance from the target 15 cm; deposition rate 10 nm min-1)would give the best result (the corresponding TEM images and transmissionspectra are given in the Supporting Information as Figures S8 and S9,respectively). Furthermore, masking the rest of the active area by sputteringPt for 10 min increases the electric conductivity of the counter electrode,which improves the cell performance significantly (Supporting InformationFigure S10).
(31) The N3 dye has a higher extinction coefficient than does N719 sothat the JSC of the DSSC made of N3 is larger than that made of N719.However, N719 contains ammonium cations to remedy the TiO2 surfaceso to obtain a larger VOC than N3. Refer to, e.g., Horiuchi, T.; Miura, H.;Sumioka, K.; Uchida, S. J. Am. Chem. Soc. 2004, 126, 12218.
(32) Nakade, S.; Kanzaki, T.; Kubo, W.; Kitamura, T.; Wada, Y.;Yanagida, S. J. Phys. Chem. B 2005, 109, 3480.
(33) Boschloo, G.; Haggman, L.; Hagfeldt, A. J. Phys. Chem. B 2006,110, 13144.